- Hot search：
AS 1816.1-2007 pdf free download
AS 1816.1-2007 pdf free download.Metallic materials-Brinell hardness test Method 1 : Test method ( ISo 6506-1 : 2005 , MOD ).
This part of ISO 6506 specifies the method for the Brinell hardness test for metallic materials and is applicable up to the limit of 650 HBW.
For specific materials and/or products, particular International Standards exist (i.e. ISO 4498-1).
2 Normative references
The following referenced documents are indispensable for the application of this document. For dated references, only the edition cited applies. For undated references, the latest edition of the referenced document (including any amendments) applies.
ISO 4498-1, Sintered metal materials, excluding hardmetals — Determination of apparent hardness — Part 1:
Materials of essentially uniform section hardness
ISO 6506-2:2005, Metallic materials — Brinell hardness test — Pail 2: Verification and calibration of testing machines
ISO 6506-4, Metallic materials — Brinell hardness test — Part 4: Table of hardness values
An indenter (hardmetal ball with diameter D) is forced into the surface of a test piece and, after removal of the force F, the diameter of the indentation d left in the surface is measured.
The Bnnell hardness is proportional to the quotient obtained by dividing the test force by the curved surface area of the indentation. The indentation is assumed to retain the shape of the ball, and its surface area is calculated from the mean indentation diameter and the ball diameter.
5.1 Testing machine, capable of applying a predetermined test force or forces within the range of 9,807 N to 29.42 kN, in accordance with ISO 6506-2.
5.2 Indenter, a polished hardmetal ball, as specified in ISO 6506-2.
5.3 MeasurIng device, as specified in ISO 6506-2.
NOTE A suggested procedure for periodic checks by the user is given in Annex A.
6 Test piece
6.1 The test shall be carried out on a surface which is smooth and even, free from oxide scale, foreign matter and, in particular, free from lubricants The test piece shall have a surface finish that will allow an accurate measurement of the diameter of the indentation.
6.2 Preparation shall be carried out in such a way that any alteration of the surface, for example, due to excessive heating or cold-working, is minimized.
6.3 The thickness of the test piece shall be at least eight times the depth of indentation. Values for the minimum thickness of the test piece in relation to the mean diameter of indentation are given in Annex B.
Visible deformation at the back of the test piece can indicate that the test piece is too thin.AS 1816.1-2007 pdf free download.
All resources on this website are from the Internet. It is only for personal study and research. No one is allowed to use it for any commercial purpose. If you need, please buy the genuine standard. If there is any infringement of your copyright, please contact the webmaster in time, and I will correct it immediately.
- Maybe you like
- Latest Updates
- ISO 287-2009 pdf free download
- ISO 527-5-2009 pdf free download
- ISO 659-2009 pdf free download
- ISO 660-2009 pdf free download
- ISO 712-2009 pdf free download
- ISO 725-2009 pdf free download
- ISO 730-2009 pdf free download
- ISO 927-2009 pdf free download
- ISO 2041-2009 pdf free download
- ISO 3040-2009 pdf free download
- ISO 3506-2-2009 pdf free download
- ISO 3506-3-2009 pdf free download